Original Article Braz J Oral Sci. October|December 2010 - Volume 9, Number 4 Influence of selective acid etching on microtensile bond strength of a self-adhesive resin cement to enamel and dentin Lúcia Trazzi Prieto1, Cíntia Tereza Pimenta Araújo2 , Maria Malerba Colombi Humel2 , Eduardo José Souza-Junior1, Carlos Tadeu dos Santos Dias3, Luís Alexandre Maffei Sartini Paulillo4 1 DDS, MS student, Department of Restorative Dentistry, Piracicaba Dental School, State University of Campinas, Piracicaba, São Paulo, Brazil 2 DDS, MS, PhD student, Department of Restorative Dentistry, Piracicaba Dental School, State University of Campinas, Piracicaba, São Paulo, Brazil 3 Agronomic engineer, MS, PhD, Associate professor, Department of Exact Science, ESALQ University of São Paulo, Piracicaba, SP, Brazil 4 DDS, MS, PhD, Full professor, Department of Restorative Dentistry, Piracicaba Dental School, State University of Campinas, São Paulo, Piracicaba, Brazil Abstract Aim: To evaluate the acid selective etching of enamel and dentin on microtensile bond strength (µTBS) of a self-adhesive resin cement. Methods: Forty-eight bovine teeth were selected and had the buccal surface ground to obtain a flat dentin (n=24) or enamel (n=24) surface. Z250 composite resin blocks (4 x 3 x 8 mm) were prepared for cementation at enamel and dentin. Each substrate received three experimental resin cementation strategies: 1) 37% phosphoric acid etching before the application of RelyX Unicem; 2) application of RelyX Unicem alone; 3) RelyX ARC as a control. Samples were light-cured using a halogen light (Optilux 501, 700mW/cm2), for 40 s. Hourglass-shaped specimens were obtained and submitted to a tensile strength at a crosshead speed of 0.5 mm/min in a universal testing machine. For statistical analysis, data were submitted to ANOVA and Tukey’s test at a pre-set alpha (á=0.05). Results: RelyX Unicem showed similar bond strength value (16.5 MPa) when compared to the pretreatment with acid etching (11.9 Mpa) and to the conventional resin cement (18.1 MPa) for enamel. All luting strategies presented similar dentin bond strength, but significantly lower than enamel bond strength. Conclusions: Acid etching prior to RelyX Unicem application did not improve microtensile bond strength for enamel and dentin. Keywords: resin cement, bond strength, dental enamel, dentin, dental acid etching. Introduction Received for publication: June 26, 2010 Accepted: October 22, 2010 With the development of adhesive dentistry, resin luting cements have been Correspondence to: widely used due to their ability to bond indirect restorations to tooth structure 1-2. Eduardo José Souza-Junior These materials can minimize some adverse effects of direct composite restorations, Piracicaba Dental School, University of like polymerization shrinkage stress magnitude 3 and gap formation at tooth/ Campinas - UNICAMP restoration interface 4.Department of Restorative Dentistry, P.O. BOX 52 Avenida Limeira, 901, Areião,13414-903 Conventional resin luting cements require prior application of bonding systems, Piracicaba - SP - Brazil which is more susceptible to procedure errors, due to unsatisfactory adhesive curing5- Phone: 55 - 19 - 8841 5291 6 , overdrying or overwetting of the dentin for hybridization7, cement incompatibility E-mail: email@example.com to some acidic monomers of the bonding system 8-10. Self-adhesive resin cements
378were introduced in an attempt to simplify resin luting strategy, (n=8): 1) RelyX Unicem (3M/ESPE, St. Paul. MN, USA); 2)in which a single clinical step is achieved11. 37% Phosphoric acid etching (Scotchbond, 3M/ESPE) In this process, demineralization/infiltration of enamel followed by RelyX Unicem; 3) RelyX ARC, as control (3M/and dentin is expected to occur simultaneously, not requiring ESPE). Luting agents were mixed and placed according toacid etch and bond system application separately 11. Some manufacturer’s instructions. For RelyX ARC, the specimenstudies state that bond strength values of self-adhesive was acid etched, Scotchbond Multi-purpose Plus (3M/ESPE)cements are comparable to those of conventional ones 12-13. was applied followed by resin cement application. TheTherefore, bonding performance of these simplified cements composition and manufacturer’s information of the resinon smear layer-covered tooth substrate still remains a luting cements are shown in Table 1.concern14-17. Also, a chemical reaction is suggested to occur Composite resin blocks (3 mm thick, 8 mm long and 4between the self-adhesive resin cement and hydroxyapatite mm wide) were built with a microhybrid composite (Z250,(3M ESPE RelyX Unicem product profile), similar to the shade A3; 3M ESPE) into a silicon mold. Composite was light-reaction of glass ionomer cements18-19. cured for 40 s with a halogen light (Optilux 501, Kerr Corp, Notwithstanding that self-adhesive resin luting cements Orange, CA, USA, at 700mW/cm2 of irradiance) and thendo not require pretreatment of the dental substrate, acid photocured at an EDG unit for 3 min. The composite surfaceetching has been proposed for removal of the smear layer in that would be in contact to the luting cement was airbone-an attempt to enhance the interaction between the cement particle abraded with 50µm aluminum oxide particles (Asferand the enamel surfaces, thus increasing the bond strength14,20. Indústria Química Ltda, São Caetano do Sul, Brazil) for 10 s.It is not clear if pretreatment with phosphoric acid etching Then, a silane couple agent (RelyX Ceramic Primer, 3M/of enamel and dentin is really efficient, and this procedure ESPE) was applied on the composite block bonding surface.is largely questioned 11,21. Resin luting cements were applied according to the tested Since the real efficacy of selective enamel and dentin groups on enamel or dentin using manufacturer’s instructions,etching is not clear by the literature, the aim of this study and then the composite blocks were cemented.was to evaluate the effect of prior acid etching of enamel Specimens were light-cured for 40 s from the buccal,and dentin on the microtensile bond strength of a self- lingual and occlusal directions. After storage in distilled wateradhesive resin luting cement, using a total-etch resin cement for 24 h, specimens were serially sectioned perpendicular toas the control. The hypothesis tested is pretreatment with the bonding interface into slabs with a diamond saw (Isometphosphoric acid etching could increase microtensile bond 1000, Buehler, UK Ltd, Lake Bluff, IL, USA), and thenstrength of RelyX Unicem to both the dental substrates. hourglass-shaped specimens were created with a cross- sectional bonded area of approximately 1 mm2. The specimensMaterial and methods were fixed to the grips of a universal testing machine (EMIC 500, São José dos Pinhais, PR, Brazil) using a cyanoacrylate adhesive (Loctite Super Bonder Gel, Henkel, D Düsseldorf, Forty-eighty bovine incisors were selected, cleaned and Germany) and tested in tension at a crosshead speed of 0.5stored in a 0.5% chloramine T solution at 4°C for no more mm/min until failure. For statistical analysis, the obtainedthan 1 week. Roots were sectioned 1 mm below the data were analyzed (SAS 9.1, SAS Institute, Inc, NC) andcementoenamel junction using a double-faced diamond saw submitted to a two-way ANOVA and Tukey’s test at 5 % of(K.G. Sorensen, São Paulo, SP, Brazil). Then, the buccal significancesurface of half of the specimens was ground on a water-cooledmechanical polisher (Metaserv 2000, Buehler, UK Ltd, LakeBluff, IL, USA) using 320-, 600- and 1200-grit silicon carbide Resultspaper (Carbimet Disc Set, #305178180, Buehler, UK Ltd,Lake Bluff, IL, USA) in order to obtain a flat dentin area of There was no statistically significant difference in theat least 8 mm2, and the other half, to obtain a flat enamel bond strength values for the tested conditions at each toothwith the same area. substrate (p>0.05). However, significant differences were Specimens were randomly assigned into 3 experimental found between enamel and dentin, where enamel showedgroups according to the luting protocol, per tooth substrate higher microtensile bond strength means compared to dentin,Table 1. Materials used in the study with composition and manufacturer’s informationResin cements Composition Manufacturer Powder: glass fillers, silica, calcium hydroxide, self-curing initiators, pigments, 3M ESPE, St Paul, MN, USA light-curing initiators, substituted pyrimidine, peroxy compound.Liquid:RelyX Unicem(Batch #270644) methacrylated phosphoric esters, dimethacrylates, acetate, stabilizers, self- curing initiators, light-curing initiators.RelyX ARC(Batch #GU9JG) Paste A: Silane treated ceramic, Bis-GMA, TEGDMA, photoinitiators, amine, 3M ESPE, St Paul, MN, USA silane treated silica, functionalized dimethacrylate polymer.Paste B: silane treated ceramic, TEGDMA, Bis-GMA, silane treated silica, benzoil peroxide, functionalized dimethacrylate polymer.
379regarding the resin luting protocol (p>0.05). These results flow 28-30. In this work, pretreatment with phosphoric acidare shown in Table 2. etching did not affected RelyX Unicem bond strength to dentin, rejecting the tested hypothesis, maybe because noTable 2. Means and standard deviations (in MPa) of further cement penetration would occur even with openedmicrotensile bond strength for the tested groups. and plug-free dentinal tubules31-33. Thereby, the viscosity of this cement may hamper the infiltration into dentin 11 . RelyX ARC RelyX Unicem Acid Etch + RelyX UnicemEnamel 18.1 (2.0)Aa 16.5 (3.8)Aa 11.9 (6.6)Aa Collagen exposure to phosphoric acid does not seem toDentin 8.1 (3.6)Ab 9.2 (7.0)Ab 8.3 (3.7)Ab improve the bonding values of the hydrophobic auto- adhesive cement34. The exact bonding mechanism of theseMean values followed by different lowercase letters in columns and uppercaseletters in rows are significantly different (Tukey’s test; p<0.05). simplified materials remains not clarified. Thus, the results are in agreement with the literature, showing higher bond strength for enamel compared to dentin either with RelyXDiscussion ARC or RelyX Unicem regardless of pretreatment with phosphoric acid etching for the self-adhesive cement 14,20. The resin luting cements used in this study (RelyX Unicem The mechanical test used in this work to evaluate theand RelyX ARC) are broadly used on clinical practice for bond strength values was the microtensile bond test35. Somecementation of indirect restorations. Moreover, self-adhesive advantages of this methodology are easier specimen collectionresin cements have been used because of its simplified resin and uniform loading stress distribution over a small bondedluting strategy, reducing clinical steps for cementation area36-39. Sticks, dumbbell bars or hourglass shapes can beprocedure, although its bond strength it is not totally clarified5- the presentation of the microtensile specimens 40-41. Also,6,11 . tensile tests are shown to be the most common laboratory Some studies have shown that the acidity of nonrinsed tests to evaluate adhesive strength of bonding systems toacidic primers can affect enamel bond strength22-24. To improve the tooth substrate38-39,41. However, there are some limitationsenamel adhesion, selective phosphoric acid etching prior to to consider about microtensile bond strength test, as stressthe application of self-adhesives resin cements has been on the bonded interface due to the handling, cuttingsuggested14,20-21. In this work, the tested hypothesis was rejected, procedure and the way of attachment40.since pretreatment with phosphoric acid etching did not affect The use of bovine teeth could be considered a limitationenamel bond strength of the self-adhesive resin cement tested. of the present work. This substrate is not as accurate as humanFor enamel, similar microtensile bond strength values were teeth when different interactions between bond system andfound, regarding the fixing system. A possible reason for this enamel/dentin are investigated. Thus, bovine teeth were selectedfact is that RelyX Unicem would present a low pH at the because they are a suitable substrate for the testedinitial stage of polymerization. Immediately after mixing the methodology, easier to collect compared to human teeth andself-adhesive cement is very acidic, lower than pH 2 at the do not rely on ethical problems. Bovine enamel and dentinfirst curing minute, reaching at about 5 after this point, are adequate alternatives for human teeth, in adhesion tests42.according to the manufacturer. This cement only reaches a However, it has been observed that a good marginal quality is more difficult to ensure with these bovine substrates4. In thisneutral pH (at about 7). The low pH after mixing promotes sense, a successful technique in bovine teeth also tends to beonly a superficial etching, increasing slightly the surface free successful in human teeth42. Additionally, the use of bovineenergy and improving mechanical bond mechanism. However, substrate has been supported by several authors43-46.it is known that hybrid layer is not formed in this interaction In conclusion, selective acid etching did not improveand part of the adhesion of self-adhesive cements occur due microtensile bond strength of RelyX Unicem to enamel andto chemical bonding to tooth hydroxyapatite 14,20 . In this dentin. The self-adhesive resin luting cement presented highermanner, enamel prisms would be affected by phosphoric acid bond strength to enamel compared to dentin and similar valuesdeep etching, maybe interfering bond strength. It goes against when compared to a conventional dual-cured resin cement.the majority of studies14,20-21, which state that micromechanical The results of this work cannot be directly extrapolated tointeraction of resin penetration between the crystallites and clinical in vivo conditions, since clinical trials are still required.enamel rods associated with chemical bonds to hydroxyapatitecould explain the higher bond strength. These studies observedan increase on bond strength between enamel and self- Referencesadhesive cements after pretreatment with phosphoric acidetching . However, etching time, acid concentration, pH, pKa, 1. Bandeca MC, El-Mowafy O, Saade EG, Rastelli ANS, Bagnato VS,hydroxyapatite buffer potential, and orientation of enamel Porto-Neto ST. Changes on degree of conversion of dual-cure luting light-prisms may significantly affect the demineralization of cured with blue LED. Laser Physics. 2009; 19: 1050-5. 2. Faria-e-Silva AL, Moraes RR, Ogliari FA, Piva E, Martins LRM. Panaviaenamel and consequently, the bond strength 25-27. F. the role of the primer. J Oral Sci. 2009; 51: 255-9. Bonding to dentin has been referred to be a less reliable 3. Cunha LG, Alonso RCB, Pfeifer CSC, Correr-Sobrinho L, Ferracane JL,strategy, especially when compared to enamel bonding, Sinhoreti MAC. Contraction stress and physical properties development ofbecause of the intrinsic characteristics of dentin, like higher a resin-based composite irradiated using modulated curing methods at twoorganic content, variations in tubular structure and fluid C-factors levels. Dent Mater. 2008; 24: 392-8.
3904. Alonso RCB, Cunha LG, Pantoja CAS, Puppin Rontani RM, Sinhoreti B. Extension of a one-step self-etch adhesive into a multi-step adhesive. MAC. Modulated curing methods – effect on marginal and internal gap Dent Mat. 2006; 22: 533-44. formation of restorations using different restorative composites. J Biomed Mat 25. Pashley DH. The effects of acid etching on the pulpodentin complex. Oper Res Part B Appl Biomat. 2007; 82: 346-51. Dent. 1992; 17: 229-42.5. Viotti RG, Kasaz A, Pena CE, Alexandre RS, Arrais CA, Reis AF. 26. Carvalho RM, Santiago SL, Fernandes CA, Suh BI, Pashley DH. Effects of Microtensile bond strength of newself-adhesive luting agents and conventional prism orientation on tensile strength of enamel. J Adhes Dent. 2000; 2: 251-7. multistep systems. J Prosthet Dent. 2009; 102: 306-12. 27. Salz U, Mücke A, Zimmermann J, Tay FR, Pashley DH. pKa value and6. Aguiar TR, Francescantonio MD, Arrais CAG, Ambrosano GMD, Davanzo C, buffering capacity of acidic monomers commonly used in self-etching primers. Giannini M. Influence of curing mode and time on degree of conversion of one J Adhes Dent. 2006; 8: 143-50. conventional and two self-adhesive resin cements. Oper Dent. 2010; 35: 295-9. 28. Pashley DH, Sano H, Ciucchi B, Yoshiyama M, Carvalho RM. Adhesion7. Faria-e-Silva AL, Fabião MM, Sfalcin RA, de Souza Meneses M, Santos- testing of dentin bonding agents: A review. Dent Mat. 1995; 11: 117-25. Filho PC, Soares PV, et al. Bond strength of one-step adhesives under 29. Frankenberger R, Kramer N, Petschelt A. Technique sensitivity of dentin different moisture conditions. Eur J Dent. 2009; 3: 290-6. bonding: Effect of application mistakes on bond strength and marginal8. Tay FR, Pashley DH, Yiu CK, Sanares AM, Wei SH. Factors contributing adaptation. Oper Dent. 2000; 25: 324-30. to the incompatibility between simplified-step adhesives and chemically- 30. D’ARCangelo C, De Angelis F, D’Amario M, Zazzeroni S, Ciampoli C, cured or dual-cured composites. Part I. Single´step self-etching adhesive. J Caputi S. The influence of luting systems on the microtensile bond strength of Adhes Dent. 2003; 5: 27-40. dentin to indirect resin-based composite and ceramic restorations. Oper9. Giannini M, De Goes MF, NIkaido T, Shimada Y, Tagami J. Influence of Dent. 2009; 34: 328-36. activation mode of dual-cured resin composite cores and low-viscosity 31. Habelitz S, Balooch M, Marshall SJ, Balooch G, Marshall GW. In situ composite liners on bond strength to dentin treated with self-etching adhesives. atomic force microscopy of partially demineralized human dentine collagen J Adhes Dent. 2004; 6: 301-6 fibrils. J Struct Biol. 2002; 138: 227-36.10. Sanares AM, Itthagarun A, King NM, Tay FR, Pashley DH. Adverse 32. Osorio R, Erhardt MC, Pimenta LAF, Osorio E, Toledano M. EDTA treatment surface interactions between one-bottle light-cured adhesives and chemical- improves resin-dentin bond’s resistance to degradation. J Dent Res. 2005; cured composites. Dent Mat. 2001; 17: 542-6. 84: 736-40.11. Mazzitelli C, Monticelli F, Toledano M, Ferrari M, Osorio R. Dentin treatment 33. Erhardt MC, Osorio R, Toledano M. Dentin treatment with MMPs inhibitors effects on the bonding performance of self-adhesive resin cements. Eur J does not alter bond strengths to caries-affected dentin. J Dent. 2008; 36: Oral Sci. 2010; 118: 80-6. 1068-73.12. PiwowARCzyk A, Bender R, Ottl P, Lauer HC. Long-term bond between 34. Gerth HU, Dammaschke T, Zuchner H, Schafer E. Chemical analysis and dual-polymerizing cementing agents and human bond dental tissue. Dent bonding reaction of RelyX Unicem and Bifix composites – a comparative Mat. 2007; 23: 211-7. study. Dent Mat. 2006; 22: 934-41.13. Bitter K, Meyer-Lueckel H, Priehn K, Kanjuparambill JP, Neumann K, 35. Sano H, SHono T, Sonoda H, Takatsu T, Ciucchi B, Carvalho R et al. Kielbassa AM. Effect of luting agent and thermocycling on bond strengths to Relationship between surface área for adhesion and tensile bond strength – root canal dentin. Int Endod J. 2006; 39: 809-18. evaluation of a micro-tensile bond test. Dent Mater. 1994; 10: 236-40.14. De Munk J, Vargas M, Van Landuyt K, Hikita K, Lambretchts, Van Meerbeek 36. Cardoso PE, Braga RR, Carrilho MR. Evaluation of micro-tensile, shear B. Bonding of an auto-adhesive luting material to enamel and dentin. Dent and tensile tests determining the bond strength of three adhesive systems. Mat. 2004; 20: 963-71. Dent Mater. 1998; 14: 394-8.15. Goracci C, Cury AH, Cantoro A, Papacchini F, Tay FR, Ferrari M. 37. Shono Y, Ogawa T, Terashita M, Carvalho RM, Pashley EL, Pashley DH. Microtensile bond strength and interfacial properties of self-etching and self- Regional measurement of resin-dentin bonding as na array. J Dent Res. adhesive resin cements used to lute composite onlays under different seating 1999; 78: 699-705. forces. J Adhes Dent. 2006; 8: 327-35. 38. Schwartzer E, Collares FM, Ogliari FA, Leitune VCB, Samuel SMW.16. Mazzitelli C, Monticelli F, Osorio R, Casucci A, Toledano M, Ferrari M. Influence of zinf oxide-eugenol temporary cement on bond strength of an all- Effect of simulated pulpal pressure on self-adhesive cements bonding to in-one adhesive system to bovine dentin. Braz J Oral Sci. 2007; 6: 1423-7. dentin. Dent Mat. 2008; 24: 1156-63. 39. Spazzin AO, Galafassi D, Gonçalves LS, Moraes RR, Carlini-Júnior. Bonding17. Aguiar TR, Di Francescantonio M, Ambrosano GMB, Giannini M. Effect of to wet or dry deproteinized dentin: Microtensile bond strength and confocal curing mode on bond strength of self-adhesive resin luting cements to dentin. laser micromorphology analysis. Braz J Oral Sci. 2009; 8; 181-4. J Biomed Mater Res Part B: Appl Biomater. 2010; 93B: 122-7. 40. El Zohairy AA, de Gee AJ, de Jager N, van Ruijven LJ, Feilzer AJ. The18. Wilson AD, Prosser HJ, Powis DM. Mechanism of adhesion of polyelectrolyte influence of specimen attachment and dimensiono n microtensile strength. J cements to hydroxyapatite. J Dent Res. 1983; 62: 590-2. Dent Res. 2004; 83: 420-4.19. Yoshida Y, Van Meerbeek B, Nakayama Y, Snauwaert J, Hallemans L, 41. El Zohairy AA, Saber MH, Abdalla AI, Feilzer AJ. Efficacy of microtensile Lambretchs P, et al. Evidence of chemical bonding at biomaterial – hard versus microshear bond testing for evaluation of bond strength of dental tissue interfaces. J Dent Res. 2000; 79: 709-14. adhesive systems to enamel. Dent Mater. 2010; 26: 848-54.20. Hikita K, Van Meerbeek B, De Munk J, Ikeda T, Van Landuyt, Maida T, et 42. Reis A,Giannini M, Kavaguchi A, Soares CJ, Line SRP. Comparison of al. Bonding effectiveness of adhesive luting agents to enamel and dentin. microtensile bond strength to enamel and dentin of human, bovine and porcine Dent Mat. 2007; 23: 71-80. teeth. J Adhes Dent. 2004; 6: 117-21.21. Duarte Jr S, Botta AC, Meire M, Sadan A. Microtensile bond strengths and 43. Nakamichi I, Iwaru M, Fusayama T. Bovine teeth as possible substitutes in scanning electron microscopic evaluation of self-adhesive and self-etch resin the adhesion test. J Dent Res. 1983; 62: 1076-81. cements to intact and etched enamel. J Prosthet Dent. 2008; 100: 203-10. 44. Peutzfeldt A, Asmussen E. Determinants of in vitro gap formation of resin22. Moura SK, Pelizzaro A, Dal Bianco K, de Goes MF, Loguercio AD, Reis A, composites. J Dent. 2004; 32: 109-15. et al. Does the acidity of self-etching primers affect bond strength and surface 45. Correr GM, Alonso RCB, Puppin-Rontani RM, Correr-Sobrinho L, Sinhoreti morphology of enamel? J Adhes Dent. 2006; 37: 35-41. MAC. Marginal and internal adaptation of composite restorations using a23. Perdigão J, Gomes G, Gondo R, Fundingsland JW. In vitro bonding resin liner on deproteinized substrate. Acta Odontol Scand. 2005; 63: 227-32. performance of all-in-one adhesives. Part I—microtensile bond strengths. J 46. Fais LMG, Marcelo CC, Silva RHBT, Guaglianoni DG, Pinelli LAP. Human Adhes Dent. 2006; 8: 367-73. teeth versus bovine teeth: cutting effectiveness of diamond burs. Braz J Oral24. Van Landuyt KL, Peumans M, De Munk J, Lambretchs P, Van Meerbeek Sci. 2010; 9: 39-42.